#------------------------------------------------------------------------------
#$Date: 2016-02-18 14:25:00 +0200 (Thu, 18 Feb 2016) $
#$Revision: 176728 $
#$URL: svn://www.crystallography.net/cod/cif/8/10/15/8101545.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_8101545
loop_
_publ_author_name
'Schreuer, Jürgen'
_publ_section_title
;
Crystal structure of silver sulfanilate, AgH₂NC₆H4SO₃
;
_journal_issue                   3
_journal_name_full
'Zeitschrift für Kristallographie - New Crystal Structures'
_journal_page_first              311
_journal_page_last               312
_journal_volume                  214
_journal_year                    1999
_chemical_formula_structural     'Ag H2 N C6 H4 S O3'
_chemical_formula_sum            'C6 H6 Ag N O3 S'
_chemical_formula_weight         280.05
_chemical_name_common            'silver sulfanilate'
_space_group_IT_number           14
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  '-P 2ybc'
_symmetry_space_group_name_H-M   'P 1 21/c 1'
_cell_angle_alpha                90.00
_cell_angle_beta                 100.10(3)
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   9.128(2)
_cell_length_b                   8.931(2)
_cell_length_c                   9.572(2)
_cell_measurement_temperature    293(2)
_cell_volume                     768.2(3)
_diffrn_ambient_temperature      293(2)
_exptl_crystal_density_diffrn    2.421
_refine_ls_R_factor_obs          0.0234
_refine_ls_wR_factor_obs         0.0549
_cod_original_sg_symbol_H-M      'P 21/c'
_cod_database_code               8101545
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, y+1/2, -z+1/2'
'-x, -y, -z'
'x, -y-1/2, z-1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_thermal_displace_type
_atom_site_occupancy
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Ag1 Ag 0.034039(19) 0.20558(2) 0.10885(2) 0.03647(8) Uani 1 d . . .
S1 S 0.81720(5) 0.38130(6) 0.31014(5) 0.02311(11) Uani 1 d . . .
O1 O 0.87166(19) 0.23149(19) 0.2891(2) 0.0363(4) Uani 1 d . . .
O2 O 0.88628(18) 0.4936(2) 0.23154(18) 0.0352(4) Uani 1 d . . .
O3 O 0.83165(18) 0.4215(2) 0.45992(17) 0.0376(4) Uani 1 d . . .
C1 C 0.6254(2) 0.3844(2) 0.2408(2) 0.0216(3) Uani 1 d . . .
C2 C 0.5287(2) 0.4515(3) 0.3181(2) 0.0281(4) Uani 1 d . . .
C3 C 0.3778(2) 0.4590(3) 0.2635(2) 0.0291(4) Uani 1 d . . .
C4 C 0.3243(2) 0.4012(2) 0.1298(2) 0.0231(3) Uani 1 d . . .
C5 C 0.4212(2) 0.3338(3) 0.0521(2) 0.0288(4) Uani 1 d . . .
C6 C 0.5720(2) 0.3250(3) 0.1069(2) 0.0285(4) Uani 1 d . . .
N1 N 0.16910(19) 0.4100(2) 0.0737(2) 0.0275(3) Uani 1 d . . .
H1 H 0.570(3) 0.490(4) 0.409(3) 0.041(8) Uiso 1 d . . .
H2 H 0.314(3) 0.503(3) 0.314(3) 0.034(7) Uiso 1 d . . .
H3 H 0.385(4) 0.293(4) -0.040(4) 0.048(9) Uiso 1 d . . .
H4 H 0.640(4) 0.283(3) 0.054(3) 0.036(8) Uiso 1 d . . .
H5 H 0.153(3) 0.422(3) -0.015(3) 0.037(8) Uiso 1 d . . .
H6 H 0.134(3) 0.483(4) 0.117(3) 0.037(8) Uiso 1 d . . .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Ag1 N1 2.2607(19) . ?
Ag1 O3 2.4102(18) 4_465 ?
Ag1 O2 2.4613(18) 2_645 ?
Ag1 O1 2.4747(19) 1_455 ?
S1 O1 1.4536(17) . ?
S1 O3 1.4613(17) . ?
S1 O2 1.4615(17) . ?
S1 C1 1.7608(19) . ?
O1 Ag1 2.4747(19) 1_655 ?
O2 Ag1 2.4613(18) 2_655 ?
O3 Ag1 2.4102(18) 4_666 ?
C1 C2 1.384(3) . ?
C1 C6 1.393(3) . ?
C2 C3 1.386(3) . ?
C3 C4 1.387(3) . ?
C4 C5 1.389(3) . ?
C4 N1 1.427(2) . ?
C5 C6 1.386(3) . ?
